High-temperature superconductors (abbreviated high-Tc or HTS) are operatively defined as materials that behave as superconductors at temperatures above nearly -200°C (-320°F).
This is in fact the lowest temperature reachable by liquid nitrogen, one of the simplest coolant in cryogenics. All superconducting materials known at ordinary pressures currently work far below ambient temperatures and therefore require cooling. The majority of high-temperature superconductors are ceramics materials. On the other hand, Metallic superconductors usually work below -200°C: they are then called low-temperature superconductors. Metallic superconductors are also ordinary superconductors, since they were discovered and used before the high-temperature ones.
Ceramic superconductors are now becoming suitable for some practical use, but they still have many manufacturing issues and there are very few successful practical examples of employment. Most ceramics are brittle which makes the fabrication of wires from them very problematic.
The major advantage of high-temperature ceramic superconductors is that they can be cooled by using liquid nitrogen. On the other hand, metallic superconductors require usually more difficult coolants - mostly liquid helium. Unfortunately, none of high-temperature superconductors are coolable using only dry ice, and none of them works at room temperature and pressure (they work well below the lowest temperature recorded on Earth). All high-temperature superconductors require some kind of cooling systems.
The main class of high-temperature superconductors are in the class of copper oxides (only some particular copper oxides). The second class of high-temperature superconductors in the practical classification is the class of iron-based compounds. Magnesium diboride is sometimes included in high-temperature superconductors: it is relatively simple to manufacture, but it superconducts only below -230°C, which makes it unsuitable for liquid nitrogen cooling (30°C below liquid nitrogen limit). For example, it can be cooled with liquid helium, which works at much lower temperatures.
Many ceramic superconductors physically behave as superconductors of the second type.
The first high temperature superconductor was discovered in 1986, by IBM researchers Bednorz and Müller, who were awarded the Nobel Prize in Physics in 1987 "for their important break-through in the discovery of superconductivity in ceramic materials"..
Some extremely-high pressure gases are usually categorized as high-temperature superconductors by theoretical physicists. In fact, many articles on high-temperature superconductors can be found on this theoretical research on high pressure gases, which is not suitable for practical applications but only for the theoretical mathematical explanation of the superconductivity phenomenon.
- 1 History
- 2 Properties
- 3 Cuprates
- 4 Ongoing research
- 5 Theoretical models
- 6 Examples
- 7 See also
- 8 References
- 9 External links
Superconductivity was discovered by Kamerlingh Onnes in 1911, in a metal solid. Ever since, researchers have attempted to observe superconductivity at increasing temperatures with the goal of finding a room-temperature superconductor. By the late 1970s, superconductivity was observed in several metallic compounds (in particular Nb-based, such as NbTi, Nb3Sn, and Nb3Ge) at temperatures that were much higher than those for elemental metals and which could even exceed 20 K (−253.2 °C). In 1986, at the IBM research lab near Zurich, in Switzerland, Bednorz and Müller were looking for superconductivity in a new class of ceramics: the copper oxides, or cuprates. Bednorz encountered a particular copper oxide whose resistance dropped to zero at a temperature around −238 °C (35.1 K). Their results were soon confirmed by many groups, notably Paul Chu at the University of Houston and Shoji Tanaka at the University of Tokyo.
Shortly after, at Princeton University, Anderson gave the first theoretical description of these materials, based on the resonating valence bond theory, but a full understanding of these materials is still developing today. These superconductors are now known to possess a d-wave[clarification needed] pair symmetry. The first proposal that high-temperature cuprate superconductivity involves d-wave pairing was made in 1987 by Bickers, Scalapino and Scalettar, followed by three subsequent theories in 1988 by Inui, Doniach, Hirschfeld and Ruckenstein, using spin-fluctuation theory, and by Gros, Poilblanc, Rice and Zhang, and by Kotliar and Liu identifying d-wave pairing as a natural consequence of the RVB theory. The confirmation of the d-wave nature of the cuprate superconductors was made by a variety of experiments, including the direct observation of the d-wave nodes in the excitation spectrum through Angle Resolved Photoemission Spectroscopy, the observation of a half-integer flux in tunneling experiments, and indirectly from the temperature dependence of the penetration depth, specific heat and thermal conductivity.
The superconductor with the highest transition temperature is the cuprate of mercury, barium, and calcium, at around 133 K.
The origin of high-temperature superconductivity is still not clear, but it seems that instead of electron-phonon attraction mechanisms, as in conventional superconductivity, one is dealing with genuine electronic mechanisms (e.g. by antiferromagnetic correlations), and instead of conventional, purely s-wave pairing, more exotic pairing symmetries are thought to be involved (d-wave in the case of the cuprates; primarily extended s-wave, but occasionally d-wave, in the case of the iron-based superconductors). In 2014, evidence showing that fractional particles can happen in quasi two-dimensional magnetic materials, was found by EPFL scientists lending support for Anderson's theory of high-temperature superconductivity.
Unfortunately, the "High-temperature" superconductor class has had many definitions in the context of superconductivity.
The label high-Tc should be reserved for materials with critical temperatures greater than the boiling point of liquid nitrogen. However, a number of materials – including the original discovery and recently discovered pnictide superconductors – have critical temperatures below 77 K but nonetheless, are commonly referred to in publications as high-Tc class.
A substance with a critical temperature above the boiling point of liquid nitrogen, together with a high critical magnetic field and critical current density (above which superconductivity is destroyed), would greatly benefit technological applications. In magnet applications, the high critical magnetic field may prove more valuable than the high Tc itself. Some cuprates have an upper critical field of about 100 tesla. However, cuprate materials are brittle ceramics which are expensive to manufacture and not easily turned into wires or other useful shapes. Furthermore, high-temperature superconductors do not form large, continuous superconducting domains, rather clusters of microdomains within which superconductivity occurs. They are therefore unsuitable for applications requiring actual superconductive currents, such as magnets for magnetic resonance spectrometers.. For a solution to this (powders), see HTS_wire.
There has been considerable debate regarding high-temperature superconductivity coexisting with magnetic ordering in YBCO, iron-based superconductors, several ruthenocuprates and other exotic superconductors, and the search continues for other families of materials. HTS are Type-II superconductors, which allow magnetic fields to penetrate their interior in quantized units of flux, meaning that much higher magnetic fields are required to suppress superconductivity. The layered structure also gives a directional dependence to the magnetic field response.
Cuprates are layered materials, consisting of superconducting layers of copper oxide, separated by spacer layers. Cuprates generally have a structure close to that of a two-dimensional material. Their superconducting properties are determined by electrons moving within weakly coupled copper-oxide (CuO2) layers. Neighbouring layers contain ions such as lanthanum, barium, strontium, or other atoms which act to stabilize the structure and dope electrons or holes onto the copper-oxide layers. The undoped "parent" or "mother" compounds are Mott insulators with long-range antiferromagnetic order at sufficiently low temperatures. Single band models are generally considered to be enough to describe the electronic properties.
The cuprate superconductors adopt a perovskite structure. The copper-oxide planes are checkerboard lattices with squares of O2− ions with a Cu2+ ion at the centre of each square. The unit cell is rotated by 45° from these squares. Chemical formulae of superconducting materials generally contain fractional numbers to describe the doping required for superconductivity. There are several families of cuprate superconductors and they can be categorized by the elements they contain and the number of adjacent copper-oxide layers in each superconducting block. For example, YBCO and BSCCO can alternatively be referred to as Y123 and Bi2201/Bi2212/Bi2223 depending on the number of layers in each superconducting block (n). The superconducting transition temperature has been found to peak at an optimal doping value (p=0.16) and an optimal number of layers in each superconducting block, typically n=3.
Possible mechanisms for superconductivity in the cuprates continue to be the subject of considerable debate and further research. Certain aspects common to all materials have been identified. Similarities between the antiferromagnetic the low-temperature state of undoped materials and the superconducting state that emerges upon doping, primarily the dx2-y2 orbital state of the Cu2+ ions, suggest that electron-electron interactions are more significant than electron-phonon interactions in cuprates – making the superconductivity unconventional. Recent work on the Fermi surface has shown that nesting occurs at four points in the antiferromagnetic Brillouin zone where spin waves exist and that the superconducting energy gap is larger at these points. The weak isotope effects observed for most cuprates contrast with conventional superconductors that are well described by BCS theory.
Similarities and differences in the properties of hole-doped and electron doped cuprates:
- Presence of a pseudogap phase up to at least optimal doping.
- Different trends in the Uemura plot relating transition temperature to the superfluid density. The inverse square of the London penetration depth appears to be proportional to the critical temperature for a large number of underdoped cuprate superconductors, but the constant of proportionality is different for hole- and electron-doped cuprates. The linear trend implies that the physics of these materials is strongly two-dimensional.
- Universal hourglass-shaped feature in the spin excitations of cuprates measured using inelastic neutron diffraction.
- Nernst effect evident in both the superconducting and pseudogap phases.
The electronic structure of superconducting cuprates is highly anisotropic (see the crystal structure of YBCO or BSCCO). Therefore, the Fermi surface of HTSC is very close to the Fermi surface of the doped CuO2 plane (or multi-planes, in case of multi-layer cuprates) and can be presented on the 2D reciprocal space (or momentum space) of the CuO2 lattice. The typical Fermi surface within the first CuO2 Brillouin zone is sketched in Fig. 1 (left). It can be derived from the band structure calculations or measured by angle resolved photoemission spectroscopy (ARPES). Fig. 1 (right) shows the Fermi surface of BSCCO measured by ARPES. In a wide range of charge carrier concentration (doping level), in which the hole-doped HTSC are superconducting, the Fermi surface is hole-like (i.e. open, as shown in Fig. 1). This results in an inherent in-plane anisotropy of the electronic properties of HTSC.
Iron-based superconductors contain layers of iron and a pnictogen—such as arsenic or phosphorus—or a chalcogen. This is currently the family with the second highest critical temperature, behind the cuprates. Interest in their superconducting properties began in 2006 with the discovery of superconductivity in LaFePO at 4 K and gained much greater attention in 2008 after the analogous material LaFeAs(O,F) was found to superconduct at up to 43 K under pressure. The highest critical temperatures in the iron-based superconductor family exist in thin films of FeSe, where a critical temperature in excess of 100 K was reported in 2014.
Since the original discoveries several families of iron-based superconductors have emerged:
- LnFeAs(O,F) or LnFeAsO1−x (Ln=lanthanide) with Tc up to 56 K, referred to as 1111 materials. A fluoride variant of these materials was subsequently found with similar Tc values.
- (Ba,K)Fe2As2 and related materials with pairs of iron-arsenide layers, referred to as 122 compounds. Tc values range up to 38 K. These materials also superconduct when iron is replaced with cobalt.
- LiFeAs and NaFeAs with Tc up to around 20 K. These materials superconduct close to stoichiometric composition and are referred to as 111 compounds.
- FeSe with small off-stoichiometry or tellurium doping.
Most undoped iron-based superconductors show a tetragonal-orthorhombic structural phase transition followed at lower temperature by magnetic ordering, similar to the cuprate superconductors. However, they are poor metals rather than Mott insulators and have five bands at the Fermi surface rather than one. The phase diagram emerging as the iron-arsenide layers are doped is remarkably similar, with the superconducting phase close to or overlapping the magnetic phase. Strong evidence that the Tc value varies with the As-Fe-As bond angles has already emerged and shows that the optimal Tc value is obtained with undistorted FeAs4 tetrahedra. The symmetry of the pairing wavefunction is still widely debated, but an extended s-wave scenario is currently favoured.
Magnesium diboride is occasionally referred to as a high-temperature superconductor because its Tc value of 39 K is above that historically expected for BCS superconductors. However, it is more generally regarded as the highest-Tc conventional superconductor, the increased Tc resulting from two separate bands being present at the Fermi level.
All known high-Tc superconductors are Type-II superconductors. In contrast to Type-I superconductors, which expel all magnetic fields due to the Meissner effect, Type-II superconductors allow magnetic fields to penetrate their interior in quantized units of flux, creating "holes" or "tubes" of normal metallic regions in the superconducting bulk called vortices. Consequently, high-Tc superconductors can sustain much higher magnetic fields.
The structure of cuprates which are superconductors are often closely related to perovskite structure, and the structure of these compounds has been described as a distorted, oxygen deficient multi-layered perovskite structure. One of the properties of the crystal structure of oxide superconductors is an alternating multi-layer of CuO2 planes with superconductivity taking place between these layers. The more layers of CuO2, the higher Tc. This structure causes a large anisotropy in normal conducting and superconducting properties, since electrical currents are carried by holes induced in the oxygen sites of the CuO2 sheets. The electrical conduction is highly anisotropic, with a much higher conductivity parallel to the CuO2 plane than in the perpendicular direction. Generally, critical temperatures depend on the chemical compositions, cations substitutions and oxygen content. They can be classified as superstripes; i.e., particular realizations of superlattices at atomic limit made of superconducting atomic layers, wires, dots separated by spacer layers, that gives multiband and multigap superconductivity.
Cuprate of Barium and Yttrium
The Cuprate of Barium and Yttrium, YBa2Cu3O7−x (or Y123), was the first superconductor found above liquid nitrogen boiling point. There are two atoms of Barium for each atom of Yttrium. The proportions of the three different metals in the YBa2Cu3O7 superconductor are in the mole ratio of 1 to 2 to 3 for yttrium to barium to copper, respectively: this particular superconductor has also often been referred to as the 123 superconductor.
The unit cell of YBa2Cu3O7 consists of three perovskite unit cells, which is pseudocubic, nearly orthorombic. The other superconducting cuprates have another structure: they have a tetragonal cell. Each perovskite cell contains a Y or Ba atom at the center: Ba in the bottom unit cell, Y in the middle one, and Ba in the top unit cell. Thus, Y and Ba are stacked in the sequence [Ba–Y–Ba] along the c-axis. All corner sites of the unit cell are occupied by Cu, which has two different coordinations, Cu(1) and Cu(2), with respect to oxygen. There are four possible crystallographic sites for oxygen: O(1), O(2), O(3) and O(4). The coordination polyhedra of Y and Ba with respect to oxygen are different. The tripling of the perovskite unit cell leads to nine oxygen atoms, whereas YBa2Cu3O7 has seven oxygen atoms and, therefore, is referred to as an oxygen-deficient perovskite structure. The structure has a stacking of different layers: (CuO)(BaO)(CuO2)(Y)(CuO2)(BaO)(CuO). One of the key feature of the unit cell of YBa2Cu3O7−x (YBCO) is the presence of two layers of CuO2. The role of the Y plane is to serve as a spacer between two CuO2 planes. In YBCO, the Cu–O chains are known to play an important role for superconductivity. Tc is maximal near 92 K when x ≈ 0.15 and the structure is orthorhombic. Superconductivity disappears at x ≈ 0.6, where the structural transformation of YBCO occurs from orthorhombic to tetragonal.
The preparation of other cuprates is more difficult than the YBCO preparation. They also have a different crystal structure: they are tetragonal where YBCO is orthorhombic. Problems in these superconductors arise because of the existence of three or more phases having a similar layered structure. Moreover, the crystal structure of other tested cuprate superconductors are very similar. Like YBCO, the perovskite-type feature and the presence of CuO2 layers also exist in these superconductors. However, unlike YBCO, Cu–O chains are not present in these superconductors. The YBCO superconductor has an orthorhombic structure, whereas the other high-Tc superconductors have a tetragonal structure.
There are three main classes of superconducting cuprates: Bismuth-based, Tallium-based and Mercurium-based.
The second cuprate by practical importance is currently BSCCO, a compound of Bi–Sr–Ca-Cu-O. The content of bismuth and strontium creates some chemical issues. It has three superconducting phases forming a homologous series as Bi2Sr2Can−1CunO4+2n+x (n=1, 2 and 3). These three phases are Bi-2201, Bi-2212 and Bi-2223, having transition temperatures of 20, 85 and 110 K, respectively, where the numbering system represent number of atoms for Bi, Sr, Ca and Cu respectively. The two phases have a tetragonal structure which consists of two sheared crystallographic unit cells. The unit cell of these phases has double Bi–O planes which are stacked in a way that the Bi atom of one plane sits below the oxygen atom of the next consecutive plane. The Ca atom forms a layer within the interior of the CuO2 layers in both Bi-2212 and Bi-2223; there is no Ca layer in the Bi-2201 phase. The three phases differ with each other in the number of planes of copper oxide (CuO2, called cuprate); Bi-2201, Bi-2212 and Bi-2223 phases have one, two and three CuO2 planes, respectively. The c axis lattice constants of these phases increases with the number of cuprate planes (see table below). The coordination of the Cu atom is different in the three phases. The Cu atom forms an octahedral coordination with respect to oxygen atoms in the 2201 phase, whereas in 2212, the Cu atom is surrounded by five oxygen atoms in a pyramidal arrangement. In the 2223 structure, Cu has two coordinations with respect to oxygen: one Cu atom is bonded with four oxygen atoms in square planar configuration and another Cu atom is coordinated with five oxygen atoms in a pyramidal arrangement.
Cuprate of Tl–Ba–Ca: The first series of the Tl-based superconductor containing one Tl–O layer has the general formula TlBa2Can-1CunO2n+3, whereas the second series containing two Tl–O layers has a formula of Tl2Ba2Can-1CunO2n+4 with n =1, 2 and 3. In the structure of Tl2Ba2CuO6 (Tl-2201), there is one CuO2 layer with the stacking sequence (Tl–O) (Tl–O) (Ba–O) (Cu–O) (Ba–O) (Tl–O) (Tl–O). In Tl2Ba2CaCu2O8 (Tl-2212), there are two Cu–O layers with a Ca layer in between. Similar to the Tl2Ba2CuO6 structure, Tl–O layers are present outside the Ba–O layers. In Tl2Ba2Ca2Cu3O10 (Tl-2223), there are three CuO2 layers enclosing Ca layers between each of these. In Tl-based superconductors, Tc is found to increase with the increase in CuO2 layers. However, the value of Tc decreases after four CuO2 layers in TlBa2Can-1CunO2n+3, and in the Tl2Ba2Can-1CunO2n+4 compound, it decreases after three CuO2 layers.
Cuprate of Hg–Ba–Ca The crystal structure of HgBa2CuO4 (Hg-1201), HgBa2CaCu2O6 (Hg-1212) and HgBa2Ca2Cu3O8 (Hg-1223) is similar to that of Tl-1201, Tl-1212 and Tl-1223, with Hg in place of Tl. It is noteworthy that the Tc of the Hg compound (Hg-1201) containing one CuO2 layer is much larger as compared to the one-CuO2-layer compound of thallium (Tl-1201). In the Hg-based superconductor, Tc is also found to increase as the CuO2 layer increases. For Hg-1201, Hg-1212 and Hg-1223, the values of Tc are 94, 128 and the record value at ambient pressure 134 K, respectively, as shown in table below. The observation that the Tc of Hg-1223 increases to 153 K under high pressure indicates that the Tc of this compound is very sensitive to the structure of the compound.
|Name||Formula||Temperature (K)||Number of planes of CuO2
in unit cell
Preparation and Manufacturing
The simplest method for preparing ceramic superconductors is a solid-state thermochemical reaction involving mixing, calcination and sintering. The appropriate amounts of precursor powders, usually oxides and carbonates, are mixed thoroughly using a Ball mill. Solution chemistry processes such as coprecipitation, freeze-drying and sol-gel methods are alternative ways for preparing a homogeneous mixture. These powders are calcined in the temperature range from 800 °C to 950 °C for several hours. The powders are cooled, reground and calcined again. This process is repeated several times to get homogeneous material. The powders are subsequently compacted to pellets and sintered. The sintering environment such as temperature, annealing time, atmosphere and cooling rate play a very important role in getting good high-Tc superconducting materials. The YBa2Cu3O7−x compound is prepared by calcination and sintering of a homogeneous mixture of Y2O3, BaCO3 and CuO in the appropriate atomic ratio. Calcination is done at 900–950 °C, whereas sintering is done at 950 °C in an oxygen atmosphere. The oxygen stoichiometry in this material is very crucial for obtaining a superconducting YBa2Cu3O7−x compound. At the time of sintering, the semiconducting tetragonal YBa2Cu3O6 compound is formed, which, on slow cooling in oxygen atmosphere, turns into superconducting YBa2Cu3O7−x. The uptake and loss of oxygen are reversible in YBa2Cu3O7−x. A fully oxygenated orthorhombic YBa2Cu3O7−x sample can be transformed into tetragonal YBa2Cu3O6 by heating in a vacuum at temperature above 700 °C.
The preparation of Bi-, Tl- and Hg-based high-Tc superconductors is more difficult than the YBCO preparation. Problems in these superconductors arise because of the existence of three or more phases having a similar layered structure. Thus, syntactic intergrowth and defects such as stacking faults occur during synthesis and it becomes difficult to isolate a single superconducting phase. For Bi–Sr–Ca–Cu–O, it is relatively simple to prepare the Bi-2212 (Tc ≈ 85 K) phase, whereas it is very difficult to prepare a single phase of Bi-2223 (Tc ≈ 110 K). The Bi-2212 phase appears only after few hours of sintering at 860–870 °C, but the larger fraction of the Bi-2223 phase is formed after a long reaction time of more than a week at 870 °C. Although the substitution of Pb in the Bi–Sr–Ca–Cu–O compound has been found to promote the growth of the high-Tc phase, a long sintering time is still required.
The question of how superconductivity arises in high-temperature superconductors is one of the major unsolved problems of theoretical condensed matter physics. The mechanism that causes the electrons in these crystals to form pairs is not known. Despite intensive research and many promising leads, an explanation has so far eluded scientists. One reason for this is that the materials in question are generally very complex, multi-layered crystals (for example, BSCCO), making theoretical modelling difficult.
Improving the quality and variety of samples also gives rise to considerable research, both with the aim of improved characterisation of the physical properties of existing compounds, and synthesizing new materials, often with the hope of increasing Tc. Technological research focuses on making HTS materials in sufficient quantities to make their use economically viable and optimizing their properties in relation to applications.
There have been two representative theories for high-temperature or unconventional superconductivity. Firstly, weak coupling theory suggests superconductivity emerges from antiferromagnetic spin fluctuations in a doped system. According to this theory, the pairing wave function of the cuprate HTS should have a dx2-y2 symmetry. Thus, determining whether the pairing wave function has d-wave symmetry is essential to test the spin fluctuation mechanism. That is, if the HTS order parameter (pairing wave function) does not have d-wave symmetry, then a pairing mechanism related to spin fluctuations can be ruled out. (Similar arguments can be made for iron-based superconductors but the different material properties allow a different pairing symmetry.) Secondly, there was the interlayer coupling model, according to which a layered structure consisting of BCS-type (s-wave symmetry) superconductors can enhance the superconductivity by itself. By introducing an additional tunnelling interaction between each layer, this model successfully explained the anisotropic symmetry of the order parameter as well as the emergence of the HTS. Thus, in order to solve this unsettled problem, there have been numerous experiments such as photoemission spectroscopy, NMR, specific heat measurements, etc. Up to date the results were ambiguous, some reports supported the d symmetry for the HTS whereas others supported the s symmetry. This muddy situation possibly originated from the indirect nature of the experimental evidence, as well as experimental issues such as sample quality, impurity scattering, twinning, etc.
This summary makes an implicit assumption: superconductive properties can be treated by mean field theory. It also fails to mention that in addition to the superconductive gap, there is a second gap, the pseudogap. The cuprate layers are insulating, and the superconductors are doped with interlayer impurities to make them metallic. The superconductive transition temperature can be maximized by varying the dopant concentration. The simplest example is La2CuO4, which consist of alternating CuO2 and LaO layers which are insulating when pure. When 8% of the La is replaced by Sr, the latter act as dopants, contributing holes to the CuO2 layers, and making the sample metallic. The Sr impurities also act as electronic bridges, enabling interlayer coupling. Proceeding from this picture, some theories argue that the basic pairing interaction is still interaction with phonons, as in the conventional superconductors with Cooper pairs. While the undoped materials are antiferromagnetic, even a few percent of impurity dopants introduce a smaller pseudogap in the CuO2 planes which is also caused by phonons. The gap decreases with increasing charge carriers, and as it nears the superconductive gap, the latter reaches its maximum. The reason for the high transition temperature is then argued to be due to the percolating behaviour of the carriers - the carriers follow zig-zag percolative paths, largely in metallic domains in the CuO2 planes, until blocked by charge density wave domain walls, where they use dopant bridges to cross over to a metallic domain of an adjacent CuO2 plane. The transition temperature maxima are reached when the host lattice has weak bond-bending forces, which produce strong electron-phonon interactions at the interlayer dopants.
D symmetry in YBCO
An experiment based on flux quantization of a three-grain ring of YBa2Cu3O7 (YBCO) was proposed to test the symmetry of the order parameter in the HTS. The symmetry of the order parameter could best be probed at the junction interface as the Cooper pairs tunnel across a Josephson junction or weak link. It was expected that a half-integer flux, that is, a spontaneous magnetization could only occur for a junction of d symmetry superconductors. But, even if the junction experiment is the strongest method to determine the symmetry of the HTS order parameter, the results have been ambiguous. J. R. Kirtley and C. C. Tsuei thought that the ambiguous results came from the defects inside the HTS, so that they designed an experiment where both clean limit (no defects) and dirty limit (maximal defects) were considered simultaneously. In the experiment, the spontaneous magnetization was clearly observed in YBCO, which supported the d symmetry of the order parameter in YBCO. But, since YBCO is orthorhombic, it might inherently have an admixture of s symmetry. So, by tuning their technique further, they found that there was an admixture of s symmetry in YBCO within about 3%. Also, they found that there was a pure dx2-y2 order parameter symmetry in the tetragonal Tl2Ba2CuO6.
Despite all these years, the mechanism of high-Tc superconductivity is still highly controversial, mostly due to the lack of exact theoretical computations on such strongly interacting electron systems. However, most rigorous theoretical calculations, including phenomenological and diagrammatic approaches, converge on magnetic fluctuations as the pairing mechanism for these systems. The qualitative explanation is as follows:
In a superconductor, the flow of electrons cannot be resolved into individual electrons, but instead consists of many pairs of bound electrons, called Cooper pairs. In conventional superconductors, these pairs are formed when an electron moving through the material distorts the surrounding crystal lattice, which in turn attracts another electron and forms a bound pair. This is sometimes called the "water bed" effect. Each Cooper pair requires a certain minimum energy to be displaced, and if the thermal fluctuations in the crystal lattice are smaller than this energy the pair can flow without dissipating energy. This ability of the electrons to flow without resistance leads to superconductivity.
In a high-Tc superconductor, the mechanism is extremely similar to a conventional superconductor, except, in this case, phonons virtually play no role and their role is replaced by spin-density waves. Just as all known conventional superconductors are strong phonon systems, all known high-Tc superconductors are strong spin-density wave systems, within close vicinity of a magnetic transition to, for example, an antiferromagnet. When an electron moves in a high-Tc superconductor, its spin creates a spin-density wave around it. This spin-density wave in turn causes a nearby electron to fall into the spin depression created by the first electron (water-bed effect again). Hence, again, a Cooper pair is formed. When the system temperature is lowered, more spin density waves and Cooper pairs are created, eventually leading to superconductivity. Note that in high-Tc systems, as these systems are magnetic systems due to the Coulomb interaction, there is a strong Coulomb repulsion between electrons. This Coulomb repulsion prevents pairing of the Cooper pairs on the same lattice site. The pairing of the electrons occur at near-neighbor lattice sites as a result. This is the so-called d-wave pairing, where the pairing state has a node (zero) at the origin.
(in degrees Celsius)
|−78||Dry ice (Carbon dioxide) - sublimation||Coolant|
|−89||Lowest temperature recorded on Earth||Coolant|
|−196||Nitrogen - Boiling||Coolant|
|−255||Nb3Sn||Metallic low-temperature superconductors|
|−270||Helium - boiling||Coolant|
|−270||Hg (mercury: the first sc discovered)||Metallic low-temperature superconductors|
- Cooper pair
- Flux pumping
- Macroscopic quantum phenomena
- Mixed conduction
- Superconducting wire
- Superconductor classification
- Cuprate superconductors
- Timmer, John (May 2011). "25 years on, the search for higher-temp superconductors continues". Ars Technica. Archived from the original on 4 March 2012. Retrieved 2 March 2012.
- Plakida, N. High Temperature Cuprate Superconductors. p. 480. ISBN 9783642126321.
- Saunders, P. J. Ford; G. A. (2005). The rise of the superconductors. Boca Raton, Fla.: CRC Press. ISBN 9780748407729.
- Choi, Charles Q. "A New Iron Age: New class of superconductor may help pin down mysterious physics". Scientific American. Retrieved 25 October 2019.
- Ren, Zhi-An; Che, Guang-Can; Dong, Xiao-Li; Yang, Jie; Lu, Wei; Yi, Wei; Shen, Xiao-Li; Li, Zheng-Cai; Sun, Li-Ling; Zhou, Fang; Zhao, Zhong-Xian (2008). "Superconductivity and phase diagram in iron-based arsenic-oxides ReFeAsO1−δ (Re=rare-earth metal) without fluorine doping". EPL. 83 (1): 17002. arXiv:0804.2582. Bibcode:2008EL.....8317002R. doi:10.1209/0295-5075/83/17002.
- Bednorz, J. G.; Müller, K. A. (1986). "Possible high TC superconductivity in the Ba-La-Cu-O system". Zeitschrift für Physik B. 64 (2): 189–193. Bibcode:1986ZPhyB..64..189B. doi:10.1007/BF01303701.
- The Nobel Prize in Physics 1987: J. Georg Bednorz, K. Alex Müller Archived September 19, 2008, at the Wayback Machine. Nobelprize.org. Retrieved April 19, 2012.
- Nisbett, Alec (Producer) (1988). Superconductor: The race for the prize (Television Episode).
- Mourachkine, A. (2004). Room-Temperature Superconductivity. (Cambridge International Science Publishing, Cambridge. pp. cond–mat/0606187. arXiv:cond-mat/0606187. Bibcode:2006cond.mat..6187M. ISBN 978-1-904602-27-9.
- Stuart A Wolf & Vladimir Z Kresin, Eds, Novel Superconductivity, Springer (October 1987)
- Tanaka, Shoji (2001). "High temperature superconductivity: History and Outlook" (PDF). JSAP International. Archived (PDF) from the original on 16 August 2012. Retrieved 2 March 2012.
- Anderson, Philip (1987). "The Resonating valence bond state in la-2CuO-4 and superconductivity". Science. 235 (4793): 1196–1198. Bibcode:1987Sci...235.1196A. doi:10.1126/science.235.4793.1196. PMID 17818979.
- Bickers, N.E.; Scalapino, D. J.; Scalettar, R. T. (1987). "CDW and SDW mediated pairing interactions". Int. J. Mod. Phys. B. 1 (3n04): 687–695. Bibcode:1987IJMPB...1..687B. doi:10.1142/S0217979287001079.
- Inui, Masahiko; Doniach, Sebastian; Hirschfeld, Peter J.; Ruckenstein, Andrei E.; Zhao, Z.; Yang, Q.; Ni, Y.; Liu, G. (1988). "Coexistence of antiferromagnetism and superconductivity in a mean-field theory of high-Tc superconductors". Phys. Rev. B. 37 (10): 5182–5185. Bibcode:1988PhRvB..37.5182D. doi:10.1103/PhysRevB.37.5182. PMID 9943697. Archived from the original on 3 July 2013.
- Gros, Claudius; Poilblanc, Didier; Rice, T. Maurice; Zhang, F. C. (1988). "Superconductivity in correlated wavefunctions". Physica C. 153–155: 543–548. Bibcode:1988PhyC..153..543G. doi:10.1016/0921-4534(88)90715-0.
- Kotliar, Gabriel; Liu, Jialin (1988). "Superexchange mechanism and d-wave superconductivity". Physical Review B. 38 (7): 5182. Bibcode:1988PhRvB..38.5142K. doi:10.1103/PhysRevB.38.5142. PMID 9946940.
- Schilling, A.; Cantoni, M.; Guo, J. D.; Ott, H. R. (1993). "Superconductivity in the Hg-Ba-Ca-Cu-O system". Nature. 363 (6424): 56–58. Bibcode:1993Natur.363...56S. doi:10.1038/363056a0.
- Dalla Piazza, B.; Mourigal, M.; Christensen, N. B.; Nilsen, G. J.; Tregenna-Piggott, P.; Perring, T. G.; Enderle, M.; McMorrow, D. F.; Ivanov, D. A.; Rønnow, H. M. (2015). "Fractional excitations in the square-lattice quantum antiferromagnet". Nature Physics. 11 (1): 62–68. arXiv:1501.01767. Bibcode:2015NatPh..11...62D. doi:10.1038/nphys3172. PMC 4340518. PMID 25729400.
- "How electrons split: New evidence of exotic behaviors". Nanowerk. École Polytechnique Fédérale de Lausanne. 23 December 2014. Archived from the original on 23 December 2014. Retrieved 23 December 2014.
- Norman, Michael R. (2008). "Trend: High-temperature superconductivity in the iron pnictides". Physics. 1 (21): 21. Bibcode:2008PhyOJ...1...21N. doi:10.1103/Physics.1.21.
- "High-Temperature Superconductivity: The Cuprates". Devereaux group. Stanford University. Archived from the original on 15 June 2010. Retrieved 30 March 2012.
- Graser, S.; Hirschfeld, P. J.; Kopp, T.; Gutser, R.; Andersen, B. M.; Mannhart, J. (27 June 2010). "How grain boundaries limit supercurrents in high-temperature superconductors". Nature Physics. 6 (8): 609–614. arXiv:0912.4191. Bibcode:2010NatPh...6..609G. doi:10.1038/nphys1687.
- Sanna, S.; Allodi, G.; Concas, G.; Hillier, A.; Renzi, R. (2004). "Nanoscopic Coexistence of Magnetism and Superconductivity in YBa2Cu3O6+x Detected by Muon Spin Rotation". Physical Review Letters. 93 (20): 207001. arXiv:cond-mat/0403608. Bibcode:2004PhRvL..93t7001S. doi:10.1103/PhysRevLett.93.207001. PMID 15600957.
- C. Hartinger. "DFG FG 538 – Doping Dependence of Phase transitions and Ordering Phenomena in Cuprate Superconductors". Wmi.badw-muenchen.de. Archived from the original on 27 December 2008. Retrieved 29 October 2009.
- Kordyuk, A. A. (2012). "Iron-based superconductors: Magnetism, superconductivity, and electronic structure (Review Article)" (PDF). Low Temp. Phys. 38 (9): 888–899. arXiv:1209.0140. Bibcode:2012LTP....38..888K. doi:10.1063/1.4752092. Archived (PDF) from the original on 11 May 2015.
- Kamihara, Y; Hiramatsu, H; Hirano, M; Kawamura, R; Yanagi, H; Kamiya, T; Hosono, H (2006). "Iron-Based Layered Superconductor: LaOFeP". Journal of the American Chemical Society. 128 (31): 10012–10013. doi:10.1021/ja063355c. PMID 16881620.
- Kamihara, Y; Watanabe, T; Hirano, M; Hosono, H (2008). "Iron-Based Layered Superconductor La[O1−xFx]FeAs (x=0.05–0.12) with Tc =26 K". Journal of the American Chemical Society. 130 (11): 3296–3297. doi:10.1021/ja800073m. PMID 18293989.
- Takahashi, H; Igawa, K; Arii, K; Kamihara, Y; Hirano, M; Hosono, H (2008). "Superconductivity at 43 K in an iron-based layered compound LaO1-xFxFeAs". Nature. 453 (7193): 376–378. Bibcode:2008Natur.453..376T. doi:10.1038/nature06972. PMID 18432191.
- Wang, Qing-Yan; Li, Zhi; Zhang, Wen-Hao; Zhang, Zuo-Cheng; Zhang, Jin-Song; Li, Wei; Ding, Hao; Ou, Yun-Bo; Deng, Peng; Chang, Kai; Wen, Jing; Song, Can-Li; He, Ke; Jia, Jin-Feng; Ji, Shuai-Hua; Wang, Ya-Yu; Wang, Li-Li; Chen, Xi; Ma, Xu-Cun; Xue, Qi-Kun (2012). "Interface-Induced High-Temperature Superconductivity in Single Unit-Cell FeSe Films on SrTiO3". Chin. Phys. Lett. 29 (3): 037402. arXiv:1201.5694. Bibcode:2012ChPhL..29c7402W. doi:10.1088/0256-307X/29/3/037402.
- Liu, Defa; Zhang, Wenhao; Mou, Daixiang; He, Junfeng; Ou, Yun-Bo; Wang, Qing-Yan; Li, Zhi; Wang, Lili; Zhao, Lin; He, Shaolong; Peng, Yingying; Liu, Xu; Chen, Chaoyu; Yu, Li; Liu, Guodong; Dong, Xiaoli; Zhang, Jun; Chen, Chuangtian; Xu, Zuyan; Hu, Jiangping; Chen, Xi; Ma, Xucun; Xue, Qikun; Zhou, X.J. (2012). "Electronic origin of high-temperature superconductivity in single-layer FeSe superconductor". Nat. Commun. 3 (931): 931. arXiv:1202.5849. Bibcode:2012NatCo...3E.931L. doi:10.1038/ncomms1946. PMID 22760630.
- He, Shaolong; He, Junfeng; Zhang, Wenhao; Zhao, Lin; Liu, Defa; Liu, Xu; Mou, Daixiang; Ou, Yun-Bo; Wang, Qing-Yan; Li, Zhi; Wang, Lili; Peng, Yingying; Liu, Yan; Chen, Chaoyu; Yu, Li; Liu, Guodong; Dong, Xiaoli; Zhang, Jun; Chen, Chuangtian; Xu, Zuyan; Chen, Xi; Ma, Xucun; Xue, Qikun; Zhou, X. J. (2013). "Phase diagram and electronic indication of high-temperature superconductivity at 65 K in single-layer FeSe films". Nat. Mater. 12 (7): 605–610. arXiv:1207.6823. Bibcode:2013NatMa..12..605H. doi:10.1038/NMAT3648. PMID 23708329.
- Jian-Feng Ge; et al. (2014). "Superconductivity in single-layer films of FeSe with a transition temperature above 100 K". Nature Materials. 1406 (3): 285–9. arXiv:1406.3435. Bibcode:2015NatMa..14..285G. doi:10.1038/nmat4153. PMID 25419814.
- Wu, G; Xie, Y L; Chen, H; Zhong, M; Liu, R H; Shi, B C; Li, Q J; Wang, X F; Wu, T; Yan, Y J; Ying, J J; Chen, X H (2009). "Superconductivity at 56 K in Samarium-doped SrFeAsF". Journal of Physics: Condensed Matter. 21 (3): 142203. arXiv:0811.0761. Bibcode:2009JPCM...21n2203W. doi:10.1088/0953-8984/21/14/142203. PMID 21825317.
- Rotter, M; Tegel, M; Johrendt, D (2008). "Superconductivity at 38 K in the Iron Arsenide (Ba1−xKx)Fe2As2". Physical Review Letters. 101 (10): 107006. arXiv:0805.4630. Bibcode:2008PhRvL.101j7006R. doi:10.1103/PhysRevLett.101.107006. PMID 18851249.
- Sasmal, K; Lv, B; Lorenz, B; Guloy, A. M.; Chen, F; Xue, Y. Y.; Chu, C. W. (2008). "Superconducting Fe-Based Compounds (A1−xSrx)Fe2As2 with A=K and Cs with Transition Temperatures up to 37 K". Physical Review Letters. 101 (10): 107007. arXiv:0806.1301. Bibcode:2008PhRvL.101j7007S. doi:10.1103/PhysRevLett.101.107007. PMID 18851250.
- Pitcher, M. J.; Parker, D. R.; Adamson, P; Herkelrath, S. J.; Boothroyd, A. T.; Ibberson, R. M.; Brunelli, M; Clarke, S. J. (2008). "Structure and superconductivity of LiFeAs". Chemical Communications. 2008 (45): 5918–5920. arXiv:0807.2228. doi:10.1039/b813153h. PMID 19030538.
- Tapp, Joshua H.; Tang, Zhongjia; Lv, Bing; Sasmal, Kalyan; Lorenz, Bernd; Chu, Paul C. W.; Guloy, Arnold M. (2008). "LiFeAs: An intrinsic FeAs-based superconductor with Tc=18 K". Physical Review B. 78 (6): 060505. arXiv:0807.2274. Bibcode:2008PhRvB..78f0505T. doi:10.1103/PhysRevB.78.060505.
- Parker, D. R.; Pitcher, M. J.; Baker, P. J.; Franke, I; Lancaster, T; Blundell, S. J.; Clarke, S. J. (2009). "Structure, antiferromagnetism and superconductivity of the layered iron arsenide NaFeAs". Chemical Communications. 2009 (16): 2189–2191. arXiv:0810.3214. doi:10.1039/b818911k. PMID 19360189.
- Hsu, F. C.; Luo, J. Y.; Yeh, K. W.; Chen, T. K.; Huang, T. W.; Wu, P. M.; Lee, Y. C.; Huang, Y. L.; Chu, Y. Y.; Yan, D. C.; Wu, M. K. (2008). "Superconductivity in the PbO-type structure α-FeSe". Proceedings of the National Academy of Sciences of the United States of America. 105 (38): 14262–14264. Bibcode:2008PNAS..10514262H. doi:10.1073/pnas.0807325105. PMC 2531064. PMID 18776050.
- Zhao, J; Huang, Q; de la Cruz, C; Li, S; Lynn, J. W.; Chen, Y; Green, M. A.; Chen, G. F.; Li, G; Li, Z; Luo, J. L.; Wang, N. L.; Dai, P (2008). "Structural and magnetic phase diagram of CeFeAsO1−xFx and its relation to high-temperature superconductivity". Nature Materials. 7 (12): 953–959. arXiv:0806.2528. Bibcode:2008NatMa...7..953Z. doi:10.1038/nmat2315. PMID 18953342.
- Lee, Chul-Ho; Iyo, Akira; Eisaki, Hiroshi; Kito, Hijiri; Teresa Fernandez-Diaz, Maria; Ito, Toshimitsu; Kihou, Kunihiro; Matsuhata, Hirofumi; Braden, Markus; Yamada, Kazuyoshi (2008). "Effect of Structural Parameters on Superconductivity in Fluorine-Free LnFeAsO1−y (Ln=La, Nd)". Journal of the Physical Society of Japan. 77 (8): 083704. arXiv:0806.3821. Bibcode:2008JPSJ...77h3704L. doi:10.1143/JPSJ.77.083704.
- Preuss, Paul. "A Most Unusual Superconductor and How It Works". Berkeley Lab. Archived from the original on 3 July 2012. Retrieved 12 March 2012.
- Hebard, A. F.; Rosseinsky, M. J.; Haddon, R. C.; Murphy, D. W.; Glarum, S. H.; Palstra, T. T. M.; Ramirez, A. P.; Kortan, A. R. (1991). "Superconductivity at 18 K in potassium-doped C60" (PDF). Nature. 350 (6319): 600–601. Bibcode:1991Natur.350..600H. doi:10.1038/350600a0.
- Ganin, A. Y.; Takabayashi, Y; Khimyak, Y. Z.; Margadonna, S; Tamai, A; Rosseinsky, M. J.; Prassides, K (2008). "Bulk superconductivity at 38 K in a molecular system". Nature Materials. 7 (5): 367–71. Bibcode:2008NatMa...7..367G. doi:10.1038/nmat2179. PMID 18425134.
- Hazen, R.; Finger, L.; Angel, R.; Prewitt, C.; Ross, N.; Mao, H.; Hadidiacos, C.; Hor, P.; Meng, R.; Chu, C. (1987). "Crystallographic description of phases in the Y-Ba-Cu-O superconductor". Physical Review B. 35 (13): 7238–7241. Bibcode:1987PhRvB..35.7238H. doi:10.1103/PhysRevB.35.7238. PMID 9941012.
- Khare, Neeraj (2003). Handbook of High-Temperature Superconductor Electronics. CRC Press. ISBN 978-0-8247-0823-8.
- Dekker, Marcel (28 September 1993). Hermann, Allen M.; Yakhmi, J.V. (eds.). Thallium-Based High-Temperature Superconductors. ISBN 9780824791148.
- Hazen, R.; Prewitt, C.; Angel, R.; Ross, N.; Finger, L.; Hadidiacos, C.; Veblen, D.; Heaney, P.; Hor, P.; Meng, R.; Sun, Y.; Wang, Y.; Xue, Y.; Huang, Z.; Gao, L.; Bechtold, J.; Chu, C. (1988). "Superconductivity in the high-Tc Bi-Ca-Sr-Cu-O system: Phase identification". Physical Review Letters. 60 (12): 1174–1177. Bibcode:1988PhRvL..60.1174H. doi:10.1103/PhysRevLett.60.1174. PMID 10037960.
- Tarascon, J.; McKinnon, W.; Barboux, P.; Hwang, D.; Bagley, B.; Greene, L.; Hull, G.; Lepage, Y.; Stoffel, N.; Giroud, M. (1988). "Preparation, structure, and properties of the superconducting cuprate series Bi2Sr2Can−1CunOy with n=1, 2, and 3" (PDF). Physical Review B. 38 (13): 8885–8892. Bibcode:1988PhRvB..38.8885T. doi:10.1103/PhysRevB.38.8885. PMID 9945668.
- Sheng, Z. Z.; Hermann, A. M.; El Ali, A; Almasan, C; Estrada, J; Datta, T; Matson, R. J. (1988). "Superconductivity at 90 K in the Tl-Ba-Cu-O system". Physical Review Letters. 60 (10): 937–940. Bibcode:1988PhRvL..60..937S. doi:10.1103/PhysRevLett.60.937. PMID 10037895.
- Sheng, Z. Z.; Hermann, A. M. (1988). "Superconductivity in the rare-earth-free Tl-Ba-Cu-O system above liquid-nitrogen temperature". Nature. 332 (6159): 55–58. Bibcode:1988Natur.332...55S. doi:10.1038/332055a0.
- Putilin, S. N.; Antipov, E. V.; Chmaissem, O.; Marezio, M. (1993). "Superconductivity at 94 K in HgBa2Cu04+δ". Nature. 362 (6417): 226–228. Bibcode:1993Natur.362..226P. doi:10.1038/362226a0.
- Schilling, A.; Cantoni, M.; Guo, J. D.; Ott, H. R. (1993). "Superconductivity above 130 K in the Hg–Ba–Ca–Cu–O system". Nature. 363 (6424): 56–58. Bibcode:1993Natur.363...56S. doi:10.1038/363056a0.
- Chu, C. W.; Gao, L.; Chen, F.; Huang, Z. J.; Meng, R. L.; Xue, Y. Y. (1993). "Superconductivity above 150 K in HgBa2Ca2Cu3O8+δ at high pressures". Nature. 365 (6444): 323–325. Bibcode:1993Natur.365..323C. doi:10.1038/365323a0.
- Shi, Donglu; Boley, Mark S.; Chen, J. G.; Xu, Ming; Vandervoort, K.; Liao, Y. X.; Zangvil, A.; Akujieze, Justin; Segre, Carlo (1989). "Origin of enhanced growth of the 110 K superconducting phase by Pb doping in the Bi-Sr-Ca-Cu-O system". Applied Physics Letters. 55 (7): 699. Bibcode:1989ApPhL..55..699S. doi:10.1063/1.101573.
- Monthoux, P.; Balatsky, A.; Pines, D. (1992). "Weak-coupling theory of high-temperature superconductivity in the antiferromagnetically correlated copper oxides". Physical Review B. 46 (22): 14803–14817. Bibcode:1992PhRvB..4614803M. doi:10.1103/PhysRevB.46.14803.
- Chakravarty, S; Sudbø, A; Anderson, P. W.; Strong, S (1993). "Interlayer Tunneling and Gap Anisotropy in High-Temperature Superconductors". Science. 261 (5119): 337–340. Bibcode:1993Sci...261..337C. doi:10.1126/science.261.5119.337. PMID 17836845.
- Phillips, J. (2010). "Percolative theories of strongly disordered ceramic high-temperature superconductors". Proceedings of the National Academy of Sciences of the United States of America. 43 (4): 1307–10. Bibcode:2010PNAS..107.1307P. doi:10.1073/pnas.0913002107. PMC 2824359. PMID 20080578.
- Geshkenbein, V.; Larkin, A.; Barone, A. (1987). "Vortices with half magnetic flux quanta in heavy-fermion superconductors". Physical Review B. 36 (1): 235–238. Bibcode:1987PhRvB..36..235G. doi:10.1103/PhysRevB.36.235. PMID 9942041.
- Kirtley, J. R.; Tsuei, C. C.; Sun, J. Z.; Chi, C. C.; Yu-Jahnes, Lock See; Gupta, A.; Rupp, M.; Ketchen, M. B. (1995). "Symmetry of the order parameter in the high-Tc superconductor YBa2Cu3O7−δ". Nature. 373 (6511): 225–228. Bibcode:1995Natur.373..225K. doi:10.1038/373225a0.
- Kirtley, J. R.; Tsuei, C. C.; Ariando, A.; Verwijs, C. J. M.; Harkema, S.; Hilgenkamp, H. (2006). "Angle-resolved phase-sensitive determination of the in-plane gap symmetry in YBa2Cu3O7−δ". Nature Physics. 2 (3): 190–194. Bibcode:2006NatPh...2..190K. doi:10.1038/nphys215.
- Tsuei, C. C.; Kirtley, J. R.; Ren, Z. F.; Wang, J. H.; Raffy, H.; Li, Z. Z. (1997). "Pure dx2-y2 order-parameter symmetry in the tetragonal superconductor Tl2Ba2CuO6+δ". Nature. 387 (6632): 481–483. Bibcode:1997Natur.387..481T. doi:10.1038/387481a0.
- High temperature superconductivity research at Cornell University
- Superconductor Science and Technology
- American Superconductor and Consolidaded Edison laying first superconductor grid in New York
- Video of a magnet floating on a HTSC
- High-Temperature Superconductor Technologies
- High-Temperature Superconductivity in Cuprates (2002) Book
- New LaOFeAs HTS SciAm